Concrete Durability towards corrosion risk – Protection strategyapplied on the Rion-Antirion Bridge ProjectL. Harikiopoulou - CordovaDesign Coordinator for Concrete and Geotechnics, Rion-Antirion ProjectP. PapanikolasTechnical Manager, Rion-Antirion ProjectS. LykoudisLaboratory Manager, Rion-Antirion ProjectKey Words: durability, slag, cover, chloride, diffusion coefficientABSTRACT: The long-term performance of concrete structures in a marine environment iscontrolled by the penetration of chlorides and the subsequent electromechanical corrosion ofembedded steel. In Rion-Antirion Bridge Project, a lifetime of 120 years is required (ref.1). Toachieve this requirement two strategies exist: (i) to postpone the penetration of chloride by relyingon concrete quality and proper cover, or (ii) to use cathodic protection of reinforcement bars. Forthe Rion-Antirion Bridge, due to the size of the concrete structures, the former strategy (concretedurability approach) has been selected.1 CONCRETE QUALITY & DURABILITY REQUIREMENTSIn order to achieve the long-term performance of 120 years of reinforced concrete structures of thebridge, it has been very important to properly characterise and evaluate the ability of the concreteto protect the embedded steel from corrosion.Three major degradation risks on reinforced concrete are due to the chemical attack by seawater,the corrosion induced by chlorides and the corrosion induced by CO2.The strategy of the concrete durability approach to protect the steel relied mainly on a properdefinition of the exposure zones, selection of appropriate concrete covers for each zone, and aproper characterisation and evaluation of concrete itself.1.1 Exposure ZonesThe structure had been split into several parts, which are:- Pile Viaducts Foundations (bored or composite)- Substructure externally exposed below MSL +10divided in: - immersed zone below MSL –5- tidal & splash zone between MSL –5 & MSL +10- Substructure externally exposed above MSL +10- Substructure overland- Bridge and Viaducts Superstructure
The most exposed zones in terms of corrosion risk are the structures externally exposed belowMSL + 10. The immersed zone (below MSL -5.0) is much less critical than the splash and tidalzone (between MSL -5.0 and MSL +10.0), due to the lack of oxygen in this area.1.2 Definition of coversThe different covers of the structure have been defined in accordance to the durability criteriaselected. As a result, higher cover than contractually required has been selected (for the sameexposure zone), especially in critical zones. Table 1 summarises the covers selected for the Rion-Antirion Bridge and applied throughout construction for the different exposure zones. Acomparison with the contractual specifications shows that in the ‘immersed zone’ and ‘tidal andsplash zone’ the cover has been increased by 20% and 13%, respectively.1.3 Concrete specifications towards durabilityIn the same way, concrete specifications higher than those required by the TCC and the KME havebeen imposed in order to achieve the requirements of concrete durability.Table 1 : Contractual Concrete specifications towards durability (as per KME and TCC)compared to Project specifications in relation to the exposure zonesNote 1: For cable-stayed bridgeNote 2: Where:- Cem III is blast furnace slag cement Cem III/A 42.5 from TITAN with 60% to 64% ofslag.- Cem II is Cem II/B-M (W-P-LL) 32.5 N from TITAN.- Cem I is Cem I 52.5 of TITAN.ExposureSituationContractualMinimumConcreteClassMinimumConcreteClassusedContractMinimumCover(mm)MinimumCoverused(mm)ContractMinimumW/C RatioMinimum W/CRatiousedContractualMinimumCementcontent(kg/m3)MinimumCementcontentused 2(kg/m3)Viaducts PileFoundationsC25/30 C25/30 - 100 0.50 0.50 360CEM II orCEM III400Immersed zone(below MSL –5)C35/45 C45/55 50 60 0.40 0.40 400CEM III400Tidal & Splash(MSL –5 to MSL +10m)C35/45 C45/55 75 85 0.40 0.40 400CEM III420Substructure externallyexposed above MSL +10C30/37 C45/55 50 50 0.45 0.40 360 CEM III400Substructure over land C30/37 C30/37 45 50 0.45 0.45 360CEM III orCEM II400Deck lowerfree surfaceC30/37 C30/37C60/75 1 40 40 0.450.450.40 1 360CEM I &CEM III400Bridge&ViaductSuperstructureDeck uppersurfaceC30/37C30/37C60/75 1 30 30 0.45 0.450.40 1360CEM I &CEM III400
Those specifications refer mainly on the choice of type of cement, the content of cement and theWater/Cement Ratio, according to the exposure situation of each part of the structure, with specialspecifications for marine environment. Table 1 gives the values of the different parameters asspecified in the KME, and as finally used on site.Based on experience gained, it is important to notice that the use of slag cement (CEM III) at ahigh quantity (> 400 kg/m3) combined with a low W/C ratio (< 0,4) in the most unfavourablezones is the most appropriate protection against corrosion risk.2 VALIDATION OF CONCRETE SPECIFICATIONS AND SET UP OF REQUIREMENTSFurther to the previous definitions, the following strategy has been developed for the bridgeproject concrete control.1) Specific tests related to durability of concrete have been defined and performed systematicallyat KG Laboratory for all mixes used in the project. Acceptance criteria have been chosen forthose tests based on experience.2) A simultaneous validation of the long-term performance of the critical areas concrete mixeshas been undertaken by LERM laboratory.3) Some additional tests on critical areas concrete mixes have been performed in KG laboratoryto satisfy experts requirements.2.1 General concrete requirements and results – All zonesFor all exposure zones, the main durability indicator has been selected to be the RCPT result(Rapid Chloride Penetration Test), combined with the WDP (Water Penetration Test) (Cf. ref.7)Those two tests have been performed systematically on all Conformity Trials for each differentmix defined for the structure.Then the respect of the fresh concrete parameters within acceptable tolerances defined in TrialMix Reports, guarantees results on hardened concrete (strength and durability characteristics)equivalent to the ones obtained during those conformity trials.The acceptance criteria for those tests have been chosen so that:- WDP ≤ 20mm- RCPT at 90 days ≤ 1000C in the splash zone≤ 2000C for substructures≤ 4000C for piles-foundations and Bridge & Viaduct superstructure(TQ 60465/0)2.2 Validation of long-term performance of concrete used in structures externally exposed belowMSL +10 (Immersed and Splash & Tidal Zones)For this particular zone, the most exposed to corrosion risk, a most precise analysis has beenperformed to verify that concrete mixes complying with the previous requirements achieveadequate long-term performance. A complete study has been entrusted to LERM Laboratory (cf.Ref.9 and Ref. 10).
2.2.1 MeasurementsMeasurements of Oxygen Permeability (AFPC-AFREM method), as well as chloride diffusioncoefficient (TANG LUPINGs method) have been performed on cores taken on walls cast in sitelaboratory with concrete mixes aimed to be used on immersed and tidal and splash zones. Thecores were taken and tested at different ages.More particularly, measurements presented in 2ndLERM report (ref 10) have been performed oncores taken from walls cast with 425 formula of C45/55 (see following table 3), cured 3 days withwater, and then installed in splash and tidal zone on site. The scope was to simulate concrete castin situ (cone, pier shaft), and exposed in splash and tidal zone at a very early age (probably theworst situation).2.2.2 Numerical SimulationsThe results obtained at different ages on concrete blocks, combined with the chloride bindingcapacity of the cement paste have been used as input data in a finite element model using a generalequation for the evolution of the diffusion coefficient with time (Cf. Ref10):D = 1.10-12t-αwith α=0,4297.This equation being determined with the help of the values measured, and the experience of LERMin similar projects as the Vasco de Gama Bridge in Portugal.2.2.3 InterpretationThose simulations lead to the presentation of chloride profiles in concrete at chosen dates, and atthe requested 120 years.On the same time, conservative and strict chloride threshold values (corrosion initiation) atreinforcement level has been defined based on experience and bibliography. The chloridethreshold at the level of reinforcement (corrosion initiation) is about 0,4 % for immersion andairborne zones, whereas it is about 0,2 % in splash and tidal zones.The superposition of the chloride profiles obtained with this threshold has allowed the validationof the long-term performance (120 years) of the Rion-Antirion Bridge Project concrete.2.3 Other TestsTaking into account Professor Gjorv advice on Durability Approach, some further tests have beenperformed on the mixes aimed to be used in immersed and splash zones, in order to reinforce theopinion of the experts on the long-term performance of this concrete.The tests performed at KG laboratory are the following:- Capillary and porosity tests (Cf. Ref 11)- Resistivity measurements (use of RCPT test)3 TEST RESULTS3.1 Laboratory resultsLaboratory results correspond to test results obtained during Trial Mixes in KG Laboratory, or atLERM premises. Anyhow, all cores and samples tested were coming from concrete cast forlaboratory purposes at the Site Batching Plant under same conditions as during regular production.
3.1.1 RCPT and WDP ResultsTable 2 summarises the RCPT and WDP Results of the principal mixes used on site:Table 2 RCPT and WDP of all concrete mixes used on siteClass ofConcreteUse of Mix Exposure Class Cement(kg/m3)D Max(mm)W/CRatioRCPT Resultsmin-max(Coulombs)WDP Resultmin-max(mm)C45/55 Main bridge footingAntirion & RionViaductSubstructure inSplash zoneSubstructure externallyexposed below MSL +10(immersed zone belowMSL –5) and SplashZoneCem III40020 0,40-0,42480-1040 2-10C45/55 Cone & pier-shaftPier Head In SituBored piles inSplash zoneImmersed zone belowMSL –5Splash & tidal zone (MSL–5 to MSL +10)Cem III42020 0,39 220-600 0-1C45/55 Mass Concrete inDry Dock and Insitu (Pier Head)Immersed zone (belowMSL –5) & Substructureexposed above MSL +10Cem III45010 0,39 450-500 1-2C50/60 Pylon Base Substructure externallyexposed above MSL +10Cem III42020 0,37 200-360 1C60/75 Pier shaft slab Splash zone (MSL –5/MSL +10)Cem III49020 0,33 220-390 5-10C60/75 Pylon legs Superstructure of MainBridgeCem III327Cem I16320 0,33 270-575 3-4C60/75Silica Fume30 kg/m3Pylon legs Superstructure of MainBridgeCem III228Cem I22820 0,37 530-710 -C60/75 Deck on shore Superstructure of MainBridgeCem III49020 0,33 320-370 5C60/75 Deck off shore Superstructure of MainBridgeCem I45020 0,33 1000-3500 at 30days-C30/37C35/45Antirion & RionViaductSubstructureSubstructure overland Cem III40020 0,44 700-1490 5-8C30/37 Composite piles forviaductsViaduct piles foundations Cem II40020 0,39 910-1380 8C40/50 Antirion Viaductprestessed beam &slabsBridge and ViaductsSuperstructureCem III140 - 150Cem I280 - 30010 0,4 1420-2900 2-6C25/30 Rion Viaduct boredpilesViaduct Piles foundations Cem III40020 0,5 1060-1420 20
It is important to notice that the results obtained are all complying with the previously definedrequirements, and most particularly in the immersed and splash zone, those results are excellent,with RCPT values significantly lower than 1000 C.3.1.2 LERM Study Resultsa) Measurements- The oxygen permeability has been measured to be < 1.10-17m2at 28 days- The chloride diffusivity has been measured to be < 1.10-12m2/s at 28 days and < 5.10-13m2/safter 4 months.Those results show already a good ability of concrete to prevent from chloride migration. On thesame time, the chloride binding capacity of the cement paste has been evaluated (Cf. Ref9)The results show that the capacity of chloride fixation by the binder is very high, approximately 50% of the total chlorides present in the paste.b) Numerical SimulationsTable 3 hereafter presents the evolution of the diffusion coefficient with time used in thesimulations, with an extrapolation of the experimental results up to 100 years thanks to theevolution law presented in paragraph 4.2.1b).Table 3 Chloride diffusion coefficient with timeTime (month) D (m2/s)0 - 1 month 5.10-121 1.10-12*4 5.10-13*12 4.10-13*120 1.10-131200 5.10-14*measured valuesThe results show an important decrease of the diffusion coefficient with time, which will lead togood long-term performance of the concrete.c) Conclusions of the StudyThese simulations gave the chloride profiles in concrete at 10 years and at 120 years in immersionand airborne zones, as well as in splash and tidal zones. They also show the relative position of thereinforcement bars according to the cover chosen. For those simulations, the value of the chloridediffusion coefficient D = 1.10-13m2/s at 10 years (see Table 3) has been used, although thedecrease of this coefficient is less significant after 10 years. The value, therefore, taken for thecalculations is conservative. Figure 1 and Figure 2 give the evolution of the chloride profiles withrespect to the location of the external reinforcement (cover), taking into account the evolution ofthe diffusion coefficient with time.
(a) Immersion and airborne zone (b) Splash and tidal zoneFigure 1 Simulation of Chloride Profiles at 10 (ref. 10 LER00003/0)(a) Immersion and airborne zone (b) Splash and tidal zoneFigure 2 Simulation of Chloride Profiles at 10 and 120 years (ref. 10 LER00003/0)The chloride profiles of Figure 2 indicate then that the diffusion coefficients determined for thoseconcrete mixes comply with the durability requirement of 120 years with regard to the corrosionrisk, provided that the value of the diffusion coefficient reaches a long-term (about 10 years) valueof D = 1.10-13m2/s.In conclusion, the tests and the simulations performed by LERM confirmed that the required lowlevel of diffusion coefficient can be obtained with the use of low W/C ratio combined with slagcement (for which compactness increases with time).
3.1.3 Other TestsThe main results on the capillary and porosity tests, as well as the resistivity measurements arepresented in Table 4.Table 4 Additional KG laboratory testsClass ofConcreteUse of Mix Exposure Class Type ofCementW/CRatioResistivitymin-max(Ohm.m))CapillaryNumber Kmin-max(kg/m2/s-0,5)CapillaryResistanceNumber M min-max (s/m2)SuctionPorosity(%)C45/55 Pier Base Raftsand PrecastslabsSubstructure externallyexposed below MSL +10(immersed zone belowMSL –5)Cem III400kg/m30,4 360 - 750 1.0 E 10-21.4 E 10-27.5 E 1062.6 E 1079.313.0C45/55 Rafts, Walls,Footing Top slabin Dry DockAntirion & RionViaductSubstructure inSplash zoneSubstructure externallyexposed below MSL +10(immersed zone belowMSL –5) and SplashZone (MSL -5 to MSL+10)Cem III400kg/m30,4 350 - 640 9.0 E 10-31.3 E 10-21.2 E 1072.0 E 1078.511.8C45/55 Cone at WetDockOctogone In SituPier Head In SituRion Viaductbored piles inSplash zoneImmersed zone belowMSL –5Splash & tidal zone (MSL–5 to MSL +10)Cem III420kg/m3< 0,4 380 - 680 9.0 E 10-31.2 E 10-28.0 E 1061.7 E 1078.110.6C45/55 Mass Concrete inDry Dock and Insitu (Pier Head)Immersed zone (belowMSL –5) & Substructureexternally exposedabove MSL +10Cem III450kg/m30,39 470 - 600 1.3 E 10-22.0 E 10-21.3 E 1071.5 E 107220.127.116.11 Adequacy of Site ResultsAll the previous "laboratory" results show a very good ability of concrete to protect embeddedsteel from corrosion.It is important at that point to notice that in Rion-Antirion Bridge Project, the extended qualitycontrol of concrete during production is the main guarantee of the compliance of the in-situconcrete with the laboratory concrete.For this reason, during mix design and conformity trial mixes (Cf. Ref. 8) performed at batchingplant, parameters of fresh concrete such as workability indicators (slump and flow) are fixed foreach formula within narrow acceptable ranges. The achievement of hardened concretecharacteristics and properties of in-situ concrete similar to those obtained during the trials areguaranteed by this way.
Those parameters are then systematically checked during concrete production at the batching plant,and concrete placement on site, and concrete is rejected if not complying with values fixed at mixdesign. (cf. Ref. 13)Furthermore, during concrete production at the batching plant, concrete is first checked by theoperators via the wattmeter (the acceptable ranges are also fixed at mix design for each formula).Then, the presence of the laboratory is necessary for any modification on the formula (ex. Watercontent), which guarantees once more good regularity of concrete produced.Finally, concrete results obtained all along the production up to now show adequacy of theconcrete produced for permanent works with the one performed for the laboratory.On the other hand, good workmanship is well prepared and controlled under Works MethodsStatements and Inspections and Tests Schedules defined precisely for each part of the structure thespecific mix design, the curing process, the minimum cover, e.t.a.Curing of concrete on site, for instance, is carefully followed up, especially in critical zones.Nevertheless, in order to verify the adequacy of laboratory concrete with in-situ one, some coringhas been punctually performed on selected by the Supervision Engineer part of structures of theBridge (which appeared not to be perfectly made or cured) and the RCPT values have beenchecked. The results are presented in Table 5.Table 5 Coring from actual production concrete poursThose results show a perfect compliance of the production concrete with the laboratory results.Finally, it is also important to notice that cover is also carefully controlled on site before casting ofstructure parts, and also after formwork removal via a covermeter on random areas, and whereverdifficulties or problems have been met before and/or during casting. From a design point of viewtwo values of concrete cover are specified: the actual minimum value (value assumed in thedesign) and the nominal minimum cover (used during construction) which is 10 mm larger in orderMixNo.StructureReferenceDate ofcastingExposure Zone RCPT Resultson productionsamplesRCPTLaboratoryresults on thesame formula406 M4.40.RAFT8.2.2. 7/12/99 Immersed Zone(below MSL - 5.0)697 480 - 1050429 M3.40.RB1M3.40.WET26M3.40.WET2511/04/0016/03/0028/03/00Immersed Zone(below MSL - 5.0)670-763-786733635-590650 - 1040446 M3.45. OC. 1-2 16/07/01 Splash Zone(between MSL -5.0 and MSL+10.0)351-390-341 450 - 500
to account for construction tolerances. This provides an additional level of security the minimumcover obtained during construction.4 CONCLUSIONS AND SUBSEQUENT FOLLOW-UPConcrete results obtained at laboratory and on site show a very good ability of Rion - AntirionBridge concrete to protect the embedded steel from corrosion, and guarantee the achievement of aservice life of 120 years.It has been, however, decided to follow-up the concrete in-situ with testing similar to the oneperformed by LERM, in order to confirm its quality towards durability requirements directly, andhence obtain more results allowing the verification of service life assessment.4.1 Validation of long-term performance of chloride diffusion coefficientAdditional cores have been taken in the walls cast for the initial durability study and installed insplash zone. They will be used by LERM in order to perform additional measures of DiffusionCoefficient, at later ages. Additional "real" points will be then added in the evolution curve andreinforce the assumption on the “α” value of the equation of evolution of the Diffusion coefficient,and hence on its long-term value.4.2 Validation of uniformity of in-situ concrete quality compared to laboratory concreteNon-destructive testing will be performed on the 4 piers in splash zone: several methods will beused to get precision in the results (radar, sclerometry, resistivity measurements). This will lead inthe determination of low, medium and high compacity areas.Then, a few cores (3 per zone) will be extracted from those areas and tested through a programsimilar to the one performed on laboratory samples in LERM. At least 3 zones (low, medium, andhigh compacity zones) will be selected in one pier, and 2 zones (low and medium compacity) onthe others.Additional cores shall also be taken to perform RCPT tests at KG laboratory.4.3 Comparison of real chloride ingress and simulated valuesDuring the construction phase, it is also proposed to cast reinforced concrete panels in-situ, similarin dimension to the ones cast for durability study in laboratory. Those panels will be cast duringreal pour of structural concrete with the same formula, and the same concrete staff, and kept underthe same conditions as real structure. Those panels will allow performing measurements of the realchloride ingress at different ages, even after the construction period. Those ages will be proposedby LERM. Those concrete panels could also be used to obtain additional points in the evolutioncurve of Diffusion Coefficient, and reinforce again the equation proposed by the LERM. The exactprogram of testing shall be defined at a later stage, and be included in the Maintenance Manual ofthe Bridge.